BULETINUL INSTITUTULUI POLITEHNIC DIN IAŞI
Universitatea Tehnică „Gheorghe Asachi” din Iaşi
Tomul LX (LXIV), Fasc. 4, 2014
EXPERIMENTAL DETERMINATION OF MECHANICAL
PROPERTIES OF AUTOCLAVED AERATED CONCRETE
MASONRY WITH VERTICAL HOLLOWS CONFINED WITH
DISPERSE REIN-FORCED CONCRETE
RĂZVAN-ANDREI IERNUŢAN* and
Technical University of Cluj-Napoca
Faculty of Civil Engineering
Received: November 19, 2014
Accepted for publication: December 10, 2014
Abstract. The present paper aims at finding solutions alternative to the
conventionally reinforced masonry, namely by replacing the confination with
reinforced concrete columns and girders with vertical and horizontal hollows in
the autoclaved aerated concrete (AAC) masonry. The voids are filled with
disperse steel fibre reinforced concrete.
The use of the disperse reinforced concrete in structural masonry walls, in
low seismic areas, is seen to allow the replacement of confined or reinforced
concrete masonry, erected according to present-day standards. A substantial
advantage can be reached, then, in areas where reinforcing transport and shaping
is difficult to achieve. In this way, buildings of type P (groundfloor)+1,2 levels
will be easier to built.
The principles of the present research concern the experimental
determination of the mechanical characteristics of masonry sections made from
AAC blocks with vertical hollows, confined with disperse reinforced concrete. A
comparison was made between findings in the unreinforced concrete sections
and masonry sections made with vertical hollows, confined with disperse
reinforced concrete; for this purpose, shear, bending and compression strength
tests were carried out on both types of sections of masonry and eventually the
modulus of elasticity of every form of masonry was determined.
*Corresponding author: e-mail: Razvan.Iernutan@ccm.utcluj.ro
88 Răzvan-Andrei Iernuţan and Maria-Nicoleta Roman-Pintican
Key words: steel fibre; force; unit stress; specific deformation.
The novelty of the research concerns the use of disperse reinforced
concrete masonry and respectively mortars in erecting structural masonry walls.
Mention should be made that there is a lack of research in civil engineering with
respect to the masonry made with disperse reinforced concrete confined hollows
(Madularu & Pop, 2010; Pop & Madularu, 2009).
Tests were performed in the Laboratory of the Faculty of Civil
Engineering from Cluj-Napoca in the interval November 2013-March 2014.
The samples were tested with a hydraulic press. A 1000 KN gauge was
used to measure forces, for data recording an HBM Spider 8 data acquisition
system was used, connected to a laptop with a special data recording and
retrieval software, namely Catman Easy.
2. The Experimental Determination of the Masonry Shear Strength, in the
2.1. Determination of Characteristic Unit Shear Strength of the Masonry
The initial characteristic unit shear strength of the masonry subjected to
unit compression stress is equal to zero fvk0 and it was found from the results of
the tests on the masonry; the reference standard used was SR EN 1052-3:2003.
In this standard, it is established determination method for the initial shear
strength in the horizontal masonry joints, where a section of masonry is
subjected to shear (CR6, 2013; SR EN 771, 2005).
The initial shear strength of the masonry was deduced from the strength
of the masonry sections subjected to stress until ultimate breaking.
The initial shear strength is defined by the linear regression curve for a
The materials used for the masonry are:
The moisture content in the silico-lime masonry member weight and for
AAC masonry member is in conformance with SR EN 772-10 (SR EN 772–1,
2005; CR6, 2013).
The mortar used fulfilled the requirements for the mixing procedure and
scattering values, according to SR EN 998-2 provisions. The mortar used was
similar to that in compression test masonry, namely M2,5.
Samples of fresh mortar were taken, in specimens of 40 × 40 × 160 mm
and the average compression strength was calculated in the moment masonry
sections were tested, according to SR EN 1015-11(CR6, 2013; SR EN 771,
Bul. Inst. Polit. Iaşi, t. LX (LXIV), f. 4, 2014 89
2.2. Preparation and Preservation of Masonry Sections
Three unreinforced masonry sections and three metal fibre reinforced
concrete masonry sections were built according to the provisions in SR EN
To determine the shear strength of the masonry, a hydraulic press to
which a spherical joint and a force gauge were mounted (Fig. 1), connected to a
data acquisition system (Fig. 2).
Fig. 1 – Sections made from
unreinforced BCA masonry.
Fig. 2 – Sections made from confined disperse
reinforced concrete BCA masonry.
ls = 300 mm
tbj = 10 mm
h2 = (h1 – tbj)/2 = 95 mm.
2.3. Preservation and Conditioning of Masonry Sections
The masonry sections were tested at 28 days and the mortar resistance
to compression was also tested at 28 days, according to SR EN 1015-11.
Positioning the masonry section in the test machine
The extremities of the masonry section were supported on the test
machine (see Fig. 3) with minimum 12 mm thick steel plates, well polished
where necessary, for a tighter contact. The load ball diameter should be 12 mm
and the minimal length of tu .
The load was applied in the middle of the top steel plate mounted on
90 Răzvan-Andrei Iernuţan and Maria-Nicoleta Roman-Pintican
a) unreinforced masonry;
b) metal fibre reinforced concrete masonry.
Fig. 3 – Testing the metal fiber reinforced concrete masonry.
2.4. Interpretation of Results
In unreinforced masonry, in all three samples, the failure occurred
between the mortar and the masonry stone, while in BFM masonry (steel fibre
reinforced concrete) the failure occurred when the member cracked until final
detachment (GP-075-02, 2003).
Fig. 4 – The failure of the metal fiber reinforced concrete masonry.
The shear strength and precompression stress were calculated for every
masonry section with a precision of 0.01 N/mm2, using the formulas below:
a) unreinforced concrete masonry – average values
ƒνoi = Fi,max /2Ai = 0.038 N/mm2, (1)
Bul. Inst. Polit. Iaşi, t. LX (LXIV), f. 4, 2014 91
b) metal fibre reinforced concrete masonry – average values
ƒνoi = Fi,max /2Ai = 0.74 N/ mm2. (2)
Fig. 5 – Evaluation of results, comparative graph (force-time) between unreinforced
masonry sections and confined disperse reinforced concrete masonry sections.
3. Experimental Bending Strength of BCA Masonry
3.1. Building BCA Masonry Sections
There were made five sections of unreinforced masonry of the
dimensions listed as follows: length ls = 91 cm, height hs= 75 cm, thickness
ts = 30 cm; the masonry was made with AAC blocks of GBN50 type of sizes:
lu = 600 mm, hu = 250 mm and tu = 300 mm; the masonry mortar used was
M2,5; the joint was 10 mm.
Other sections with a vertical hollow were built of size 200 x 200 mm to
confine the disperse steel fibre reinforced concrete masonry. The dimensions of
this masonry section are identical to those of unreinforced sections. The sections
were built from AAC, of the dimensions: lu = 600 mm, hu = 250 mm and tu =
= 300 mm; the M2,5 masonry mortar was used and joints were of 10 mm. In the
vertical hollows, concrete of grade C16/20 was poured; it was built with steel
fibres of type WHS 50/09/H. The concrete formula comes in agreement with the
Standard NE–12/1–2007(Normativ pentru producerea betonului şi executarea
lucrărilor din beton, beton armat şi beton precomprimat/ Norms for producing
concrete and performing concrete, reinforced concrete and presstressed concrete
works) and the Guildelines GP-075-02 „Ghid pentru stabilirea criteriilor de
performanta şi a compoziţiilor pentru betoanele armate dispers cu fibre
metalice”/ Guildelines to establish performance criteria and composition of
disperse metal fibre reinforced concrete (Pop & Madularu, 2008; GP-075-02,
2003; SR EN 1052–3, 2003).
92 Răzvan-Andrei Iernuţan and Maria-Nicoleta Roman-Pintican
Fig. 6 – Building the vertical hollow masonry section.
3.2. Testing BCA Masonry for Resistance to Bending
After mounting the samples in the test location, the load test was
uniformly distributed on the two supports placed on the masonry section.
The sample bending stress test was performed with a hydraulic cylinder
mounted perpendicularly to the masonry wall. A metal profile stand was also
In order to assess the deformations, every masonry section was
provided with two comparison mechanical gauges, arranged as shown in the
Figs. 7 and 8.
Fig. 7 – The bending strength of
unreinforced masonry test.
Fig. 8 – The